159

Volume 64 18 Number 1, 2016

http://dx.doi.org/10.11118/actaun201664010159

## TENSILE STRENGTH OF THE EGGSHELL

## MEMBRANES

### Jana Strnková

1_{, Šárka Nedomová}

1_{, Vojtěch Kumbár}

2_{, Jan Trnka}

3
1_{ Department of Food Technology, Faculty of AgriSciences, Mendel University in Brno, Zemědělská 1, 613 00 Brno, }
Czech Republic

2_{ Department of Technology and Automobile Transport, Faculty of AgriSciences, Mendel University in Brno, }
Zemědělská 1, 613 00 Brno, Czech Republic

3_{ Institute of Thermomechanics, Czech Academy of Science, Dolejškova 5, 182 00 Praha, Czech Republic}

**Abstract**

STRNKOVÁ JANA, NEDOMOVÁ ŠÁRKA, KUMBÁR VOJTĚCH, TRNKA JAN. 2016. Tensile
Strength of the Eggshell Membranes. *Acta Universitatis Agriculturae et Silviculturae Mendelianae Brunensis,*
64(1): 159–164.

The mechanical behaviour of eggshell membranes under tensile loading has been studied. Samples
from diﬀ erent bird species (hen, goose and Japanese quail) have been used. Samples were cut out
of the membrane in latitudinal direction. TIRAtest 27025 tensile testing machine equipped with
a 200 N load-cell was used. Tensile deformation exhibits both non-linear as well as linear region.
The experiments were performed at ﬁ ve loading velocities 1, 10, 100, 400 and 800 mm.min−1_{. The main }

parameters describing the eggshell strength increase with the loading rate. This dependence exhibits the same qualitative features as the rate dependence of the eggshell strength.

Keywords: eggshell membrane, tensile test, loading rate, tensile strength, fracture strain

**INTRODUCTION**

Eggshell membrane is a part of egg which adheres
to eggshell, but its eﬀ ect on eggshell strength
is still not clear because there is not any way to
research eggshell membrane with intact eggshell
and it is o en considered as an unimportant
impact factor on eggshell strength. Only limited
number of information is known about its physical
and structural properties, such as the pore and
mechanical characteristics of the membrane.
The only exception represents the paper of
Torres *et al.* (2010) which is focused on the study of
hen’s egg membranes under tensile loading and
nanoindentation.

The given paper is focused on the research of
the eggshell membranes behaviour under tensile
loading. The results on the fracture strength of
the whole eggshell show that this parameter is more
or less dependent on the loading rate (Carter, 1979;
Trnka *et al.,* 2012; Nedomová *et al.,* 2014). The same
dependence may occur also for the eggshell
membranes. In the given paper this dependence
has been studied on the eggshell membranes of
three domestic fowls (hen, goose and Japanese
quail). The knowledge of these characteristics is

meaningful e.g. in design of the numerical model
of egg. These models are than used in numerical
simulation of the egg behaviour under diﬀ erent
loads (Song *et al.,* 2006; Perianu *et al.,* 2010).

**MATERIALS AND METHODS**

27025 tensile testing machine equipped with
a 200 N load-cell was used. Rectangular samples
(15 mm × 15 mm) were used for the measurements.
The results obtained were statistically analyzed
using the statistical package UNISTAT. Evaluated
were the means and standard deviations using
ANOVA with subsequent Tukey’s test at signiﬁ cance
level of *P *> 0.95. Thickness of the membranes
exhibits a scatter as shown in the Fig. 1.

The statistical analysis shows that statistically signiﬁ cant diﬀ erence occurs between thickness of goose and quail eggshell membranes. Histogram of this quantity is displayed in the Fig. 2.

Statistical data are given in the Tab. I.

Specimens were glued to thin metallic plates – see Fig. 3.

1: *Membrane thickness (On each box, the central mark is the median, the edges of the box are the 25th _{ and 75}th_{ percentiles, the whiskers extend }*

*to the most extreme data points not considered outliers, and outliers are plotted individually)*

2: *Histogram of the membrane thickness (broken lines denote a fitted normal distribution)*

I: *Membrane thickness*

**Thickness [mm]** **Minimum** **Mean** **Maximum** **Standard deviation**

Hen’s egg 0.022 0.080 0.170 0.037

Goose’s egg 0.033 0.070 0.110 0.025

Quail’s egg 0.040 0.062 0.090 0.014

The deformation of the sample was assumed
to be equal to the separation of the crossheads.
The force *F *and the deformation *l = l − lo*, where

*l* is the instantaneous specimen length at the time
*t*, are measured during tension and both quantities
are recorded. The force-deformation data may
easily be transformed into normalized quantities
such as stress and strain. The Cauchy strain and
Hencky’s natural or true strain are of common use
in representing compression curves. The evaluation
of these quantities as well as the values of stress, ,
and/or true stress, respectively is described e.g. by
Mehnet Ak and Gunasekaran (1997).

The specimen deformation is also described using the stretching parameter, , which is deﬁ ned as

*C*
*o*

*l*
*l* 1

. (1)

The transformation force-deformation data into
quantities given above have been performed using
of MATLAB so ware. Five speeds, *v*, were used: 1,
10, 100, 400 and 800 mm.min−1_{. Loading rate can be }

converted to the strain rate:

*o*

*d* *v*

*dt* *l*

_{ }_{}

. (2)

The corresponding values of strain rates
are: 0.00111; 0.0111; 0.111; 0.444 and 0.888 s−1_{. }

Experiments were performed at the room
temperature. Experimental data for Japanese quails
were published independently in (Strnková *et al.,*
2015).

**RESULTS AND DISCUSSION**

In the Fig. 4 an example of the experimental record force-displacements is shown.

The loading force increases up to some value corresponding to the membrane fracture. In this moment the force nearly immediately falls to zero. The only exceptions were observed

for the membranes of quail eggs. The force decreases gradually in this case. This is probably a consequence of relatively low crack velocity in the membrane.

Experimental records force-displacement
were converted to the dependence of stress, ,
on the strain, , using of Eqs. in Mehnet Ak and
Gunasekaran (1997). The maximum of the stress
corresponds to the moment of eggshell membrane
fracture. This quantity is denoted as the ultimate
tensile strength (UTS). The corresponding
strain represents the fracture strain * _{f}*. The next
parameter which describes the fracture behaviour
of the eggshell membrane is the fracture toughness.
This quantity is expressed as the energy absorbed by
the eggshell membrane up to rupture point per unit
volume of the membrane and was determined using
the following formula (Polat

*et al.,*2007):

*f*

*W* *d*

0

_{}

. (3)
Experimental data describing the eggshell membrane fracture behaviour are given in the Tabs. II–IV.

These data show that all fracture parameters in-crease with the loading velocity. These dependences are shown in the Fig. 5.

The dependence of the ultimate tensile strength on the loading velocity v can be ﬁ tted by the power function:

*UTS* = *a* + *bvc*_{. (4)}

The parameters of Eq. 4 are given in the Tab. V. The same function can be used for the ﬁ tting of experimental data on the fracture toughness. The corresponding coeﬃ cients are given in the Tab. VI.

The power function (4) can be also used for the
ﬁ tting of data on the fracture strain *f*for quail and

hen eggs. The coeﬃ cients are given in the Tab. VII.

For the goose eggs the inﬂ uence of loading rate on the fracture strain can be described by a linear function:

*f* = *a* + *bv*, (5)

where *a* = 0.2942, *b* = 0.0003018 min.mm−1_{ and }

R2_{ = 0.9332.}

The statistical analysis of the obtained data was
performed at loading rates 1, 10, 100 and 800 mm.
min−1_{. The results are presented in the Tabs. VIII–X.}

With exception of the smallest loading velocity,
*v* = 1 mm.min−1, the fracture parameters UTS,

*f*

and *W* increase from quail eggshell membranes
towards to the goose eggshell membranes. The same
tendency has been observed for the fracture
parameters of the eggshells in our previous papers.
II: *Fracture parameters of the eggshell membranes (Japanese quail eggs)*

**Loading rate** **Ultimate tensile strength [MPa]**

**Minimum** **Mean** **Maximum** **Standard deviation**

1 mm.min−1 _{1.05} _{1.11} _{1.15} _{0.04}

10 mm.min−1 _{2.09} _{2.16} _{2.24} _{0.06}

100 mm.min−1 _{2.80} _{2.95} _{3.08} _{0.11}

800 mm.min−1 _{3.57} _{3.74} _{3.91} _{0.14}

**Fracture strain [1]**

**Minimum** **Mean** **Maximum** **Standard deviation**

1 mm.min−1 _{0.184} _{0.204} _{0.247} _{0.025}

10 mm.min−1 _{0.242} _{0.281} _{0.311} _{0.026}

100 mm.min−1 _{0.339} _{0.352} _{0.373} _{0.014}

800 mm.min−1 _{0.387} _{0.408} _{0.421} _{0.013}

**Fracture toughness [J/m3 _{]}**

**Minimum** **Mean** **Maximum** **Standard deviation**

1 mm.min−1 _{ 76874.22} _{ 91869.40} _{128544.59} _{20844.65}

10 mm.min−1 _{340874.07} _{362883.64} _{376454.47} _{13293.23}

100 mm.min−1 _{389065.19} _{462359.97} _{486152.42} _{41308.33}

800 mm.min−1 _{664204.87} _{686757.33} _{704406.12} _{15044.17}

III: *Fracture parameters of the eggshell membranes (goose eggs)*

**Loading rate** **Ultimate tensile strength [MPa]**

**Minimum** **Mean** **Maximum** **Standard deviation**

1 mm.min−1 _{1.920071} _{1.971661} _{2.014312} _{0.034015}

10 mm.min−1 _{2.529502} _{2.583293} _{2.624702} _{0.035093}

100 mm.min−1 _{2.634261} _{2.788316} _{2.920022} _{0.103276}

400 mm.min−1 _{3.766396} _{3.839524} _{3.910143} _{0.053282}

800 mm.min−1 _{4.313467} _{5.041023} _{5.751289} _{0.528752}

**Fracture strain [1]**

**Minimum** **Mean** **Maximum** **Standard deviation**

1 mm.min−1 _{0.244090} _{0.250444} _{0.256095} _{0.005268}

10 mm.min−1 _{0.319801} _{0.326091} _{0.329823} _{0.004730}

100 mm.min−1 _{0.322989} _{0.339340} _{0.357237} _{0.013624}

400 mm.min−1 _{0.411308} _{0.419686} _{0.428123} _{0.006762}

800 mm.min−1 _{0.525468} _{0.531089} _{0.537910} _{0.005045}

**Fracture toughness [J/m3 _{]}**

**Minimum** **Mean** **Maximum** **Standard deviation**

1 mm.min−1 _{347362} _{351519} _{354109} _{2743}

10 mm.min−1 _{693398} _{710578} _{747518} _{21783}

100 mm.min−1 _{1184200} _{1223068} _{1245695} _{23050}

400 mm.min−1 _{2120673} _{2160572} _{2284200} _{69764}

IV: *Fracture parameters of the eggshell membranes (hen eggs)*

**Loading rate** **Ultimate tensile strength [MPa]**

**Minimum** **Mean** **Maximum** **Standard deviation**

1 mm.min−1 _{0.870474} _{0.973065} _{1.088092} _{0.087483}

10 mm.min−1 _{1.826440} _{1.848202} _{1.888617} _{0.027697}

100 mm.min−1 _{2.176184} _{2.340416} _{2.455979} _{0.102541}

400 mm.min−1 _{2.549244} _{2.603649} _{2.681369} _{0.056045}

800 mm.min−1 _{3.093290} _{3.223861} _{3.380857} _{0.124523}

**Fracture strain [1]**

**Minimum** **Mean** **Maximum** **Standard deviation**

1 mm.min−1 _{0.293602} _{0.303027} _{0.317544} _{0.010220}

10 mm.min−1 _{0.220139} _{0.231636} _{0.246372} _{0.010196}

100 mm.min−1 _{0.167102} _{0.279578} _{0.189587} _{0.008846}

400 mm.min−1 _{0.335579} _{0.344040} _{0.358985} _{0.009004}

800 mm.min−1 _{0.400034} _{0.411178} _{0.419943} _{0.007172}

**Fracture toughness [J/m3 _{]}**

**Minimum** **Mean** **Maximum** **Standard deviation**

1 mm.min−1 _{0.181875} _{0.196750} _{0.208750} _{0.010573}

10 mm.min−1 _{0.246250} _{0.260713} _{0.279375} _{0.012874}

100 mm.min−1 _{0.341250} _{0.354007} _{0.373750} _{0.013866}

400 mm.min−1 _{0.398750} _{0.410682} _{0.431875} _{0.012752}

800 mm.min−1 _{0.491875} _{0.508625} _{0.521875} _{0.010802}

5: *Main fracture parameters of tested eggshell membranes*

V: *Coeﬃ cients in equation (8), UTS vs. v, (R2 _{ denotes the correlation)}*

**Eggshell **

**membrane** **a [MPa]** **b [MPa]** **c [1]** **R2**

Quail 10.37 −9.239 −0.0493 0.9957

Goose 2.17 0.025 0.7088 0.9764

Hen −20.55 21.580 0.0133 0.9617

VI: *Coeﬃ cients in equation (8), W vs. v, (R2 _{ denotes the correlation)}*

**Eggshell **

**membrane** **a [MPa]** **b [MPa]** **c [1]** **R2**

Quail 1.163 × 106 _{−2.058 × 10}6_{−0.04779 0.9735}
Goose 2.159 × 105 _{1.672 × 10}5 _{0.40510} _{0.9927}
Hen 1.170 × 107 _{−1.161 × 10}7 _{0.00763} _{0.9915}

VII: *Coeﬃ cients in equation (8), _{f }vs. v, (R2_{ denotes the correlation)}*

**Eggshell **

**membrane** **a [MPa]** **b [MPa]** **c [1]** **R2**

Quail 0.9398 −0.7358 −0.0486 0.9999

Hen 0.2658 0.001836 1 0.8528

Goose 0.2942 0.0003018 1 0.9332

VIII: *Results of ANOVA analysis of the results on UTS, (+ denotes *
*statistically signiﬁ cant diﬀ erence, n.s denotes no signiﬁ cant diﬀ erence)*

**Loading rate [mm.min−1 _{]}**

_{1}

_{10}

_{100}

_{800}Quail – Hen n.s + + +

Hen – Goose n.s + + +

IX: *Results of ANOVA analysis of the results on the fracture strain, *
*(+ denotes statistically signiﬁ cant diﬀ erence, n.s denotes no signiﬁ cant *
*diﬀ erence)*

**Loading rate [mm.min−1 _{]}**

_{1}

_{10}

_{100}

_{800}Quail – Hen n.s + n.s +

Hen – Goose + + + +

Quail – Goose + + + +

X: *Results of ANOVA analysis of the results on the fracture *
*toughness, (+ denotes statistically signiﬁ cant diﬀ erence, n.s denotes no *
*signiﬁ cant diﬀ erence)*

**Loading rate [mm.min−1 _{]}**

_{1}

_{10}

_{100}

_{800}Quail – Hen n.s + n.s +

Hen – Goose + + + +

Quail – Goose + + + +

**CONCLUSION**

Fracture of eggshell membranes at tensile loading has been studied. The fracture behaviour can be
described in terms of the ultimate tensile strength (UTS), fracture strain (_{f}) and fracture toughness
(W). Results obtained in this paper show that these quantities increase with the loading rate. With
exception of the smallest loading velocity (1 mm.min−1_{) the values of the fracture parameters exhibit }

the smallest value for the eggshell membrane of the quail egg and the highest for the eggshell membrane of goose egg.

Acknowledgement

The authors would like to acknowledge the support of IP 17/2014 IGA MENDELU and of the Institute of Thermomechanics AS CR, v. v. i. of the Czech Academy of Sciences through institutional support No. RVO: 61388998.

**REFERENCES**

CARTER, T. C. 1979. The hen’s egg: Evidence on the
mechanism relating shell strength to loading rate.
*Brit. Poultry Sci., *20(2): 175–183.

NEDOMOVÁ, Š., BUCHAR, J. and STRNKOVÁ, J.
2014. Goose’s eggshell strength at compressive
loading. *Potravinarstvo, *8(1): 54–61.

PERIANU, C., DE KETELAERE, B., PLUYMERS,
B., ZESMET, W., DEBAERDEMAEKER, J. and
DECUYPERE, E. 2010. Finite element approach
for simulating the dynamic mechanical behaviour
of a chicken egg. *Biosyst. Eng., *106(1): 79–85.

MEHMET AK, M. and GUNASEKARAN, S. 1997.
Anisotropy in tensile properties of mozzarella
cheese. *J. Food Sci.,* 62(5): 1031–1033.

POLAT, R., TARHAN, S., ÇETIN, M. and ATAY, U. 2007. Mechanical behaviour under compression loading and some physical parameters of Japanese

quail (*Coturnix coturnix japonica*) eggs. *Czech. J. Anim. *
*Sci., *52(2): 50–56.

SONG, H. Z., WANG, J. and YE, J. A. 2006. Analysis
of the loading properties of fowl eggshell with
ﬁ nite element method. *J. Zhejiang Univ. Sci., *32(3):
350–354.

STRNKOVÁ, J., NEDOMOVÁ, Š., TRNKA, J.,
BUCHAR, J. and KUMBÁR, V. 2015. Behaviour of
eggshell membranes at tensile loading. *Bulg. Chem. *
*Commun.,* 47(special issue B): 44–48.

TORRES, F. G., TRONCOSO, O. P., PIAGGIO, F. and
HIJAR, A. 2010. Structure-property relationships
of a biopolymer network: the eggshell membrane.
*Acta Biomater*., 6(9): 3687–3693.

TRNKA, J., BUCHAR, J., SEVERA, L., NEDOMOVÁ,
Š. and STOKLASOVÁ, P. 2012. Eﬀ ect of loading
rate on hen’s eggshell mechanics. *Journal of Food *
*Research, *1(4): 96–105.

Contact information Jana Strnková: jana.strnkova@ mendelu.cz